Synthesis of Inorganic Compounds in the Matrix of Polysaccharide Chitosan

Data related to the fabrication of hybrid materials based on the polysaccharide chitosan were systematized and reviewed. The possibility of using chitosan as a “host” matrix for in situ synthesis of inorganic compounds for the preparation of various types of composite materials were investigated. Coprecipitation of metal oxides/hydroxides (Fe, Ni, Al, Zr, Cu and Mn) with chitosan was carried out through the alkalinization of solutions containing metal salts and chitosan, with the addition of ammonia or alkali solutions, homogeneous hydrolysis of urea, or electrophoretic deposition on the cathode. The synthesis of transition metal ferrocyanides and hydroxyapatite was achieved from precursor salts in a chitosan solution with simultaneous alkalinization. The mechanism of composite formation during the coprecipitation process of inorganic compounds with chitosan is discussed. Composite materials are of interest as sorbents, coatings, sensors, and precursors for the production of ceramic and electrode materials.


Introduction
Recently, there has been increasing interest in hybrid materials in which inorganic components are introduced into a polymer matrix. These materials enable advances in the fields of application of nanodispersed metal powders, metal oxides/hydroxides, and some salts for use as sorbents, catalysts, and sensors in forms acceptable for practical application, such as granules, membranes, films, and fibers [1][2][3], due to the possibility of preserving the dispersity of nanoparticles (NPs) by preventing their agglomeration and oxidation. The use of biopolymers for the immobilization of inorganic nanoparticles constitutes a new trend in the development of chemistry of nanomaterials (especially biodegradable and biocompatible ones) in various fields, particularly in biomedicine. Therefore, these biopolymer (host)/immobilized nanoparticle (guest) systems serve as a convenient medium for the realization of several chemical processes that are often unavailable under the so-called "traditional" performance conditions of chemical reactions in solutions or solid phase. Examples of these systems include gelatin-immobilized ferrocyanides (FOC) of transition metals, comprising nanoreactors for the synthesis of new compounds [4], or the gelatincalcium phosphate system [5], which can be used for creating ceramic composite materials in bone tissue engineering [5][6][7].
Chitosan-based nanomaterials are characterized by superior qualities compared to the initial chitosan as a result of the introduction of NPs of various compounds, which impart desirable properties such as high specific surface area, stability, conductivity, photoluminescence sorption properties, and improved mechanical strength [17].
Nanoparticles of inorganic compounds can be introduced to chitosan, as in synthetic polymers, through dispersion (immobilization) of pre-fabricated NPs into the polymer solution with subsequent polymer solidification. However, significantly higher interest has been devoted towards the synthesis of materials comprising nanoparticles (guests) in a biopolymer matrix simultaneously with precipitation. However, information on the synthesis of compounds directly in the chitosan matrix is rather insufficient.
The objective of the present work was to demonstrate, on the basis of several examples from the available literature and our own work, possibilities for such syntheses using chitosan as a matrix (host) for the immobilization of inorganic compounds (guests).
Morphology of the composite materials and distribution of the inorganic component in the bulk was investigated using a Lyra3 XMH (Tescan) scanning electron microscope equipped with an AZtecEnergy energy dispersive X-ray (EDX) microanalyzer automated with an X-Max80 detector (Oxford Instruments, Abingdon, UK).
The phase composition and crystallinity of resulting samples were determined by X-ray diffraction analysis (XRD) using a D8 ADVANCE diffractometer with CuKα (λ = 0.15418 nm) incident radiation and SmartLab diffractometer (Rigaku, Japan) with CuKα-radiation in the 2 θ range from 2 • to 80 • at a scan speed of 0.2 • /s. Information about some organo-mineral composites, initial reagents, and methods used for their preparation is summarized in Table 1.  [26] CFS-chitosan ferrocyanide sorbent K-Ni, K-Cu,

Sorbent for Cs
The chitosan acidic solution was combined with transition metal salt (Ni, Cu, or Zn), then the obtained mixture was dispersed to the alkaline solution of potassium ferrocyanide. Otherwise (vice versa), the alkaline solution of potassium ferrocyanide was dispersed to the chitosan acidic solution containing a Ni(II) salt. The molar ratio M 2+ /[Fe(CN) 6 ] 4-= 3:1.
The precipitate was filtered and heated at 100 • C.
Present study [27,28] HA/CS HA/CS Films, biomedical coatings, membranes The CS solution was combined with salts CaCl 2 and K 2 HPO 4 at the molar ratio Ca/P = 1.67. The mixture was placed into NH 3 atmosphere and held there for 1 h until pH~10. Then the mixture was heated at 100 • C for 12 h. Conversion of the film to by treatment with alkali 0.1 M NaOH (24 h at 95-100 • C; 72 h at room temperature).

Material Characteristics Ni(OH) 2 /CS and Ni(OH) 2 /CS/ACF
Ni(OH) 2 /CS obtained by crushing and subsequent sieving of fractions with a given particle size have an irregular shape. The particles have a dense structure. In the particles deposited on the surface of the carbon fiber, a layered structure is observed ( Figure 1). Figure 2 shows the X-ray diffraction pattern of the "gel-in-gel" synthesis products. Ni(OH) 2 in the composite sample has a characteristic XRD pattern for α-Ni(OH) 2 corresponding to a layered turbostratic structure [38].  Figure 2 shows the X-ray diffraction pattern of the "gel-in-gel" synthesis products. Ni(OH)2 in the composite sample has a characteristic XRD pattern for α-Ni(OH)2 corresponding to a layered turbostratic structure [38].

Сharacteristics of CFS-Chitosanferrocyanide Sorbent Ni-K, Cu-K, Zn-K
As an example, Figure 3 shows the SEM image of the surface of a particle of the composite sorbent CS/FOC K-Ni. The particles have a dense structure.  Figure 2 shows the X-ray diffraction pattern of the "gel-in-gel" synthesis products. Ni(OH)2 in the composite sample has a characteristic XRD pattern for α-Ni(OH)2 corresponding to a layered turbostratic structure [38].

Сharacteristics of CFS-Chitosanferrocyanide Sorbent Ni-K, Cu-K, Zn-K
As an example, Figure 3 shows the SEM image of the surface of a particle of the composite sorbent CS/FOC K-Ni. The particles have a dense structure.

Characteristics of CFS-Chitosanferrocyanide Sorbent Ni-K, Cu-K, Zn-K
As an example, Figure 3 shows the SEM image of the surface of a particle of the composite sorbent CS/FOC K-Ni. The particles have a dense structure.

Material Characteristics HA/CS.
According to the SEM image data shown in Figure 5 for HA/CS, the sample obtained in the NH3 atmosphere has a porous structure.

Material Characteristics HA/CS.
According to the SEM image data shown in Figure 5 for HA/CS, the sample obtained in the NH3 atmosphere has a porous structure.

Material Characteristics HA/CS
According to the SEM image data shown in Figure 5 for HA/CS, the sample obtained in the NH 3 atmosphere has a porous structure.

Discussion
Chitosan is a natural polysaccharide produced by N-deacetylation of chitin. As a co-polymer, chitosan is comprised of linear β-(1→4) glycosidiclinkages which are similar in structure to cellulose. In chitosan, 2-acetamido-D-glucose and 2-amino-D-glucose units are combined with glycosidic linkages [17]. Chitosan is a bio-compatible, bio-degradable, bio-renewable, and non-toxic polymer characterized with a variety of useful properties ensuring a substantial interest to hybrid materials on its basis, which can be widely applied as powders, nanoparticles, gel granules, films and membranes, sponges, fibers, or hollow fibers. However, here, the chitosan properties promoting the formation and the fabrication of various organo-inorganic materials is highlighted. The majority of natural polysaccharides, such as pectin, dextrin, agar, agarose, carrageenan, and cellulose, are naturally acidic, whereas chitosan is a highly basic polysaccharide [17].
Chitosan is a natural cationic polysaccharide. It is water-soluble and positively charged and can be obtained by protonation under acidic conditions: Chitosan properties in solutions depend on the molecular weight, degree of deacetylation, pH, and solution ionic strength. At pH 6.5, CS amino groups are deprotonated. As a result of the charge decrease along with the pH increase, the soluble chitosan usually flocculates at pH around 6.0 [39].
Additionally, the polymer could participate in formation of complex compounds consisting of a polymer as a ligand and several transition metal ions bonded to the polymer by a coordination bond [40], which can also form precipitates in alkaline media.
Thus, in alkaline media, chitosan coprecipitation with cations of some metals results in the formation of organo-inorganic composites.

Ni(OH) 2 /Chitosan Nanosize Composites
Among metal hydroxides, nickel hydroxide is most often used in advanced power devices for energy accumulation (batteries and supercapasitors) because of its high theoretical specific capacity, large interlayer distance in the layered structure, excellent pseudo-capacity properties, ease of synthesis, and stability in alkaline electrolytes [41].
Fabrication of nanostructured Ni(OH) 2 is realized through high-efficiency precipitation methods in the presence of surfactants, and also in the presence of a "green template"chitosan. The Ni(OH) 2 /CS serves here as an intermediate product in the fabrication of the mesoporous nickel hydroxide [20].
In this study, the fabrication of the Ni(OH) 2 /CS composite is based on the precipitation of nickel hydroxide from aqueous solution of Ni 2+ during the decomposition of the urea present in the solution. At a temperature of 60 • C, the urea decomposition becomes rather fast, increasing the pH under homogeneous conditions throughout the whole solution volume when precipitation of metal hydroxides becomes possible without creating a high degree of supersaturation. Here, urea acts as a "delay base", since there is no reaction when it is dissolved in the aqueous metal salt solution at room temperature. The urea hydrolysis starts when temperature increases above 333 K, in accordance with the reaction, in which hydroxide ions are released gradually into the homogeneous medium, whereas pH increases throughout the whole solution volume [38]. For nickel hydroxide, the pH of the precipitation start is in the range 6.7 to 7.7, depending on the concentration [42]. In the presence of chitosan in the solution, it is precipitated at pH > 6. Thus, the homogeneous hydrolysis results in the precipitation of the hybrid material Ni(OH) 2 /CS in the presence of chitosan as an external template. Upon the introduction of carbon fiber to the solution as a substrate, the composite is precipitated on the carbon fiber surface. Figure 2 shows the X-ray diffraction patterns of the products of synthesis of Ni(OH) 2 /CS ("gel in gel"). In the process of synthesis, nickel hydroxide precipitated in the material composition has a characteristic XRD pattern corresponding to α-Ni(OH) 2 (curve 2) with the turbostratic structure identical to the one reported in [38]. The sizes of Ni(OH) 2 crystallites contained in the hybrid material are as follows: Ni(OH) 2 /CS, 100 • C-9.48 nm; Ni(OH) 2 /CS/ACF, 100 • C-3.75 nm.
However, it is worth noting that poor reproducibility was observed in our experimental results. In repeated syntheses, compounds are formed preceding α-Ni(OH) 2 , with a maximum diffraction at 2 θ~12 • and 22 • and smaller particle sizes (curve 1). The latter could be related to the fact that colloid systems are distinguished by poor property reproducibility.
The surface morphology of the composite materials is shown in Figure 1.
Particles of oxides and hydroxides can be formed using the method of electrosynthesis most appropriate for their growth in a polymer matrix of the polyelectrolyte chitosan with precipitation of compounds or metal-polymer complexes [22][23][24][25].
Metal-containing particles in a polymer matrix were formed as a result of an electrolytic process, in which metal ions or complexes were hydrolyzed by the cathodegenerated base with precipitation of hydroxides, oxides, or other insoluble phases, in a manner dependent on the ions present in the electrolyte composition on the substrate surface [43]. The OH − -ion-generating cathode reactions are as follows: Precipitation of nanosize particles on the surface of substrates with highly developed surface and porosity is attractive in terms of using carbon fiber as a cathode. First, the rate of generation of hydroxide ions is rather high. Secondly, the composite material oxide/hydroxide/chitosan is formed as a film on the ACF surface, which is attractive for creating sorbents, electrode materials, and catalysts, in which the processes occur mostly on the material surface, rather than in its bulk.

Transition Metal Ferrocyanides/Chitosan Hybrid Sorbents
Hybrid sorbents based on transition metal ferrocyanides in a chitosan matrix are of interest for cesium removal. Chitosan used as a matrix and insoluble in alkaline media provides a certain stability for ease peptized FOC precipitates, which enables the use of FOC for decontamination in columns and the easy removal of spent sorbents from the reactive medium. The stability of transition metal FOC in the composition of hybrid sorbents applicable for the removal of cesium from high-salinity streams makes it possible to use them in cesium concentration from seawater [44].
There are different methods for the immobilization of FOC into the polysaccharide matrix. In particular, the introduction of FOC into the chitin matrix as granules [45] or foam [46] can be implemented using chitosan. The chitosan solution is added with a prepared FOC suspension, after which granules or discs are formed with subsequent freezing and lyophilic drying and reacetylation of glucosamine groups in order to form chitin.
The synthesis of transition metal ferrocyanides in a chitosan matrix is described in detail in [26][27][28]. In [26], the freshly prepared chitosan resin was saturated with copper(II) and washed, after which wet granules were placed into a solution of K 4 [Fe(CN) 6 ] with formation of the resin K 2 Cu 3 [Fe(CN) 6 ] 2 in the phase. However, to obtain a sorbent, granules (spheres) with a water content of 92-96 wt.% were used in order to saturate the resin with copper until a certain capacity. Such resins are prepared in several stages by gelling in appropriate solutions. Grains contain a lot of water, so they are difficult to store and impossible to transport at low temperatures, which limits their practical application. Fabrication of hybrid materials is significantly facilitated by simple mixing of two solutions (acidic chitosan solution containing a transition metal salt and alkaline solution of potassium fer-rocyanide) resulting in precipitation of chitosan with simultaneous synthesis of transition metal FOC in the "host" matrix [27,28].
As observed from the XRD data (Figure 4), the use of chitosan had no effect on the structural characteristics of ferrocyanides. The X-ray images correspond to those of pure FOC powders and materials formed ex situ with the introduction of preliminarily obtained particles to the polymer [45,46].

Hybrid Calcium Phosphates/Chitosan Composites
Hydroxyapatite/chitosan (HA/CS) is one of the most often synthesized composites. It can be produced by means of different techniques from the precursors of calcium salts (Ca(NO 3 ) 2 , CaCl 2 , Ca(OH) 2 , or CaCO 3 ) and orthophosphoric acid salts or orthophosphoric acid. This results in the possibility of synthesizing a complex hydroxyl-/oxyapatite composite consisting of all anions and cations from solution. Different methods have been applied for the fabrication of HA/CS composites: simultaneous coprecipitation with chitosan during ammonia [33,37] or sodium hydroxide [31,35] alkalization, lyophilized composites treatment by sodium hydroxide [32], and electrodeposition on substrate [36].
Hydrolysis of urea-phosphate (NH 2 ) 2 CO-H 3 PO 4 is of great interest because of the slow reagent introduction and solution alkalization [33,34]. Ammonia and sodium hydroxide alkalization are used to increase pH. For example, transformation of brushite into HA is carried out using NaOH. The composite fabrication is usually completed with its lyophilization, which is accompanied by the development of its porous structure [30,31].
Introduction of the calcium salt and potassium (ammonium) phosphate to the acidic chitosan solution by the stoichiometric ratio Ca/P = 1.67 results in the formation of hydroxyapatite in accordance with the following reaction [5,15], In the method we developed, alkalization of the mixture of salts and chitosan is realized by holding it, placed in a Petri dish, in an ammonia atmosphere for a long period of time. Thereafter, the precipitate is dried and heated at~100 • C. Here, hydroxyapatite is not formed, but the formation of crystalline phosphate phase with a non-apatite structure can be observed (Figure 6 curve a), with high content of ammonium chloride (reaction proceeds in HCl from calcium chloride). The transformation of this phase to hydroxyapatite was performed by treatment of the material with a 0.1 M solution of sodium hydroxide at 95-100 • C (or for 72 h at room temperature) ( Figure 6, curves b,c) [37].
Phase transformation was corroborated on the basis of the XRD analysis, Figure 6, and SEM data, Figure 5.

Conclusions
For preparation of composite organo-mineral materials based on chitosan, various methods can be used. These include the deposition and co-deposition of inorganic particles and chitosan in alkaline medium. Additionally, composite films containing oxides and hydroxides in a chitosan matrix can be obtained by cathode electrodeposition based on electrophoretic deposition of chitosan and electrosynthesis of inorganic nanoparticles.
Ultrathin nanosheets of α-Ni(OH) 2 in a chitosan matrix were synthesized by using homogeneous hydrolysis of urea at elevated temperature. In the process of increasing pH homogeneously in the bulk solution, the simultaneous formation of nickel hydroxide and chitosan gels occurs. Precipitation and subsequent drying lead to the production of the Ni(OH) 2 /CS composite.
Immobilization of transition metal ferrocyanides into a chitosan matrix to obtain effective sorbents for Cs was carried out by the precipitation method. When mixing two solutions of salts of precursors of FOC-a chitosan solution containing a transition metal salt (Ni, Cu, Zn) and an alkaline ferrocyanide solution-mixed ferrocyanides FOC M-K (M-Ni, Cu, Zn) of the required composition are formed. The composition and content of ferrocyanides in chitosan matrix can be easy controlled by changing the concentration of salts.
Biocomposite materials based on chitosan and calcium phosphates were obtained. Depending on the pH, drying and washing conditions, different phases are formed. The most suitable conditions for synthesis of the phosphate phase of non-apatite structure were homogeneous precipitation using NH 3 vapors for treatment of chitosan solution containing HA precursors at a molar ratio of Ca/P of 1.67. Hydroxyapatite as the main phosphate phase was detected after treatment of this phase with 0.1 M NaOH.